Magnetic anisotropy of a Co(II) single ion magnet with distorted trigonal prismatic coordination: theory and experiment.
Peng, Yan; Bodenstein, Tilmann; Fink, Karin; Mereacre, Valeriu; Anson, Christopher E.; Powell, Annie K.; Physical chemistry chemical physics : PCCP 18 (2016) 30135–30143; doi:10.1039/c6cp03157a

data_7226781
_publ_section_title
;
 Magnetic anisotropy of a Co(II) single ion magnet with distorted trigonal
 prismatic coordination: theory and experiment.
;
_journal_issue                   43
_journal_name_full               'Physical chemistry chemical physics : PCCP'
_journal_page_first              30135
_journal_page_last               30143
_journal_paper_doi               10.1039/c6cp03157a
_journal_volume                  18
_journal_year                    2016
_chemical_formula_moiety         'C26 H34 Co N4 O4'
_chemical_formula_sum            'C26 H34 Co N4 O4'
_chemical_formula_weight         525.50
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/6
_audit_update_record
;
2015-09-04 deposited with the CCDC.
2016-10-11 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 96.396(5)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   16.1119(11)
_cell_length_b                   7.0151(6)
_cell_length_c                   21.1805(14)
_cell_measurement_reflns_used    13381
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      26.83
_cell_measurement_theta_min      1.94
_cell_volume                     2379.1(3)
_computing_cell_refinement       'X-Area 1.38 (Stoe & Cie GmbH, 2006)'
_computing_data_collection       'WinXpose 1.6.8 (Stoe & Cie GmbH, 2004)'
_computing_data_reduction        'X-Area 1.38 (Stoe & Cie GmbH, 2006)'
_computing_molecular_graphics    'Diamond 2.1 (Crystal Impact, 1998)'
_computing_publication_material  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXT (Sheldrick, 2014)'
_diffrn_ambient_temperature      150(2)
_diffrn_detector_area_resol_mean 6.667
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Stoe IPDS II'
_diffrn_measurement_method       'area detector, \w-scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0322
_diffrn_reflns_av_unetI/netI     0.0292
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            16727
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        25.250
_diffrn_reflns_theta_max         26.342
_diffrn_reflns_theta_min         1.510
_exptl_absorpt_coefficient_mu    0.763
_exptl_absorpt_correction_T_max  0.930
_exptl_absorpt_correction_T_min  0.756
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
XPREP in SHELXTL 6.14 (BrukerAXS Inc., 2003)
;
_exptl_crystal_colour            red-brown
_exptl_crystal_density_diffrn    1.467
_exptl_crystal_description       prism
_exptl_crystal_F_000             1108
_exptl_crystal_preparation       'Magnetic properties'
_exptl_crystal_size_max          0.350
_exptl_crystal_size_mid          0.310
_exptl_crystal_size_min          0.230
_refine_diff_density_max         0.241
_refine_diff_density_min         -0.663
_refine_diff_density_rms         0.083
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.989
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     316
_refine_ls_number_reflns         4819
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.989
_refine_ls_R_factor_all          0.0415
_refine_ls_R_factor_gt           0.0326
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0609P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0842
_refine_ls_wR_factor_ref         0.0867
_reflns_Friedel_coverage         0.000
_reflns_number_gt                3898
_reflns_number_total             4819
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c6cp03157a2.cif
_cod_data_source_block           12041119
_cod_depositor_comments          'Adding full bibliography for 7226781.cif.'
_cod_database_code               7226781
_shelx_estimated_absorpt_t_min   0.776
_shelx_estimated_absorpt_t_max   0.844
_shelxl_version_number           2014/6
_shelx_res_checksum              5829